- Nano Express
- Open Access
Nanoscale characterization of electrical transport at metal/3C-SiC interfaces
© Eriksson et al; licensee Springer. 2011
Received: 1 October 2010
Accepted: 7 February 2011
Published: 7 February 2011
In this work, the transport properties of metal/3C-SiC interfaces were monitored employing a nanoscale characterization approach in combination with conventional electrical measurements. In particular, using conductive atomic force microscopy allowed demonstrating that the stacking fault is the most pervasive, electrically active extended defect at 3C-SiC(111) surfaces, and it can be electrically passivated by an ultraviolet irradiation treatment. For the Au/3C-SiC Schottky interface, a contact area dependence of the Schottky barrier height (ΦB) was found even after this passivation, indicating that there are still some electrically active defects at the interface. Improved electrical properties were observed in the case of the Pt/3C-SiC system. In this case, annealing at 500°C resulted in a reduction of the leakage current and an increase of the Schottky barrier height (from 0.77 to 1.12 eV). A structural analysis of the reaction zone carried out by transmission electron microscopy [TEM] and X-ray diffraction showed that the improved electrical properties can be attributed to a consumption of the surface layer of SiC due to silicide (Pt2Si) formation. The degradation of Schottky characteristics at higher temperatures (up to 900°C) could be ascribed to the out-diffusion and aggregation of carbon into clusters, observed by TEM analysis.
With respect to the hexagonal silicon carbide polytype (4H-SiC), cubic silicon carbide (3C-SiC) has potential advantages for power device applications, specifically in terms of higher electron mobility in metal oxide semiconductor field-effect transistor [MOSFET] channels and due to the absence of bipolar degradation upon electrical stress [1, 2]. However, the low stacking fault [SF] formation energy for this polytype  leads to high densities of these defects, which prevent the achievement of the predicted electrical properties. While 3C-SiC MOSFETs with excellent on-state characteristics have been demonstrated , a significant reduction of the SF density is required in order to achieve acceptable blocking voltage values and off-state leakage currents. Hence, it is crucial to better understand which role these defects play in the non-ideal contact properties and explore ways to mitigate their detrimental influence on devices. In this sense, imaging the evolution of the structural and electrical properties at SiC interfaces at a nanoscale level can be the way to better understand the physical transport phenomena and to finally improve the performance of potential devices.
In this work, the transport properties of metal/3C-SiC interfaces were characterized employing nanoscale techniques in combination with the conventional electrical measurements. In particular, the nanoscale electrical activity of SFs in the semiconductor at the contact interface was studied by conductive atomic force microscopy [C-AFM]. The effects of a surface passivation on the localized leakage currents through SFs and the characteristics of fabricated Au/-3C-SiC diodes were discussed. Also, the electrical and structural properties of the Pt/3C-SiC system were studied, where high-temperature annealing can induce metal/SiC interface reactions and strongly affect the barrier homogeneity and leakage currents caused by semiconductor surface states.
3C-SiC(111) heteroepitaxial 12-μm n-type ([N] = 2 × 1017 cm−3) layers were grown onto (0001) 4H-SiC substrates using a chlorine-based chemical vapor deposition [CVD] process  (sample A). Homoepitaxial 4-μm n-type ([N] = 3 × 1015 cm−3) 3C-SiC layers were grown on free-standing 3C-SiC(001) substrates  using CVD (sample B). Ohmic back contacts were formed by evaporation of a 100-nm-thick layer of Ni and a subsequent rapid annealing step at 950°C for 60 s to form nickel silicide [7, 8]. The 3C-SiC surfaces were then subjected to a UV irradiation treatment at 200°C in order to electrically passivate carbon-related defect states at the surface [9, 10]. Front contacts were formed by sputter deposition of a 100-nm-thick Au (samples A and B) or Pt film (sample B), and circular contacts with radii from 5 to 150 μm were defined by a lift-off process. The fabricated Pt diodes were annealed for 5 min at 500°C, 700°C, and 900°C in argon ambient. The structural evolution of the Pt/3C-SiC system upon thermal annealing was studied by X-ray diffraction [XRD] and transmission electron microscopy [TEM], which was also used to study structural defects in the 3C-SiC epilayers. XRD patterns were measured using a Bruker-AXS D5005 θ-θ diffractometer. TEM analyses were carried out after mechanical thinning and a final ion milling at low energy (5 keV Ar ions). Bright field images were recorded at 2-20 kV by a JEOL 2010F microscope equipped with the Gatan imaging filter. The effects of the structural evolution on the electrical behavior of fabricated Schottky diodes were investigated by current-voltage (I-V) characterization in a Karl Süss electrical probe station, as well as by C-AFM , performed using a Veeco DI dimension 3100, equipped with the nanoscope V electronics and the scanning spreading resistance [SSRM] module . The parameters describing the metal/3C-SiC interfaces were extracted from I-V measurements using thermionic emission theory .
Results and discussion
A key factor for the conduction properties through a contact is the quality of the metal/semiconductor interface, e.g., structural defects reaching the semiconductor surface can lead to a localized barrier lowering and increased leakage currents [14, 15]. It has recently been shown by SSRM mapping, performed in cross-section, that extended defects in 3C-SiC cause a localized lowering of the resistance through the layer . As a consequence, the crystalline quality of the 3C-SiC epilayer is pivotal for good device operation.
The effect of the passivation on the I-V behavior of fabricated Au/3C-SiC(111) diodes is shown in Figure 1c. A strong reduction of the leakage current is observed, while the forward current is largely unaffected. However, even after this passivation, a contact area dependence of the Schottky barrier height was observed for the Au/3C-SiC system where ΦB gradually increased from 0.7 to 1.4 eV as the contact radius was reduced from 150 to 5 μm .
The contact area dependence of ΦB observed for the Au/3C-SiC(111) system may result from an inhomogeneous interface between the metal and the semiconductor, or it could be caused by leakage currents related to surface states. Independent of its origin, this dependence should be mitigated if a 'fresh' metal/SiC interface is created instead of forming the contact interface at the original sample surface which was exposed to chemicals, sputter damage, and to air.
Pt is known to react with SiC at high temperatures, thus consuming a thin surface layer of SiC to form platinum silicide, in turn forming a new interface with the SiC. Both Pt and its silicides have high work functions that should result in good barrier heights on 3C-SiC . Hence, we investigated the properties of the Pt/3C-SiC system upon high-temperature annealing. Previous studies on Pt contacts to 3C-SiC have reported the onset of platinum silicide phase formation to occur at annealing temperatures ranging from 650°C to above 750°C [20, 21]. Moreover, both increased  and reduced [21, 23] leakage currents have been reported upon silicide phase formation. Clearly, the effects of high-temperature annealing on the structural and electrical properties of Pt/3C-SiC is ambiguous. In this study, XRD analysis (not reported here) showed that the Pt2Si phase was formed already after annealing the Pt/3C-SiC(001) system at 500°C. The Pt2Si phase is thermodynamically stable in the studied temperature range , and the XRD patterns remain essentially the same also after annealing at 700°C and 900°C. Ternary compounds are not stable, meaning that carbon must be freed during the reaction. Indeed, the XRD spectra showed an increased presence of crystalline carbon with increasing annealing temperature.
To understand the electrical evolution upon annealing, the cross-section of the contact interface was studied by TEM. As seen in the TEM images in Figure 2 the Pt layer (Figure 2a) has reacted completely after the 500°C anneal (Figure 2b), and the consumption of Pt results in the formation of a polycrystalline Pt2Si layer, characterized by the presence of interfacial protrusions penetrating into the underlying SiC . However, additional changes are observed at the higher temperatures. At 700°C (Figure 2c), larger size variations are visible in the Pt2Si protrusions and there is a formation of a carbon layer at the interface and carbon clusters inside the protrusions (also confirmed by energy-filtered TEM). After annealing at 900°C, this layer is thicker and more pronounced carbon clusters are observable inside the protrusions.
The TEM observations can be consistently correlated to the previously shown electrical results. Since Pt2Si is the only phase observed by XRD for the different annealing temperatures, the evolution of the electrical properties after annealing above 500°C is likely unrelated to the silicide phase formation. More likely, the changes in the electrical properties can be related to changes in the density of states at the contact interface. As reported by Mullins and Brunnschweiler , for the as-deposited contacts, the surface states are presumed to behave as donor-like traps, generated during the sputtering of the metal. Hence, after annealing at 500°C, the interface moves away from the original 3C-SiC surface and these states no longer affect the properties of the contact, causing a widening of the energy barrier that in turn causes the tunneling leakage current to reduce. The gradual degradation observed at higher annealing temperatures can be explained by the increased amount of carbon clusters at the contact interface and in the Pt2Si protrusions due to incomplete diffusion of carbon upon further consumption of SiC, which has been shown to become an issue at annealing above 600°C . The agglomeration of electrically active carbon clusters at the interface gives rise to barrier inhomogeneities, characterized by local low-barrier patches, ultimately leading to an increase of the leakage current .
Nanoscale electrical and structural characterization of metal/3C-SiC interfaces were performed using C-AFM, XRD, and TEM. It was shown that the most pervasive extended defect at 3C-SiC(111) surfaces, the stacking fault, can be passivated by UV irradiation treatment. This allowed an almost ideal Schottky behavior to be measured for the Au/3C-SiC system when characterizing very small diodes. However, a contact area dependence of the Schottky barrier height was found after this passivation, indicating that other electrically active defects and/or inhomogeneities at the contact interface still remain even after UV passivation. The contact area dependence of ΦB was absent for the Pt/3C-SiC system, which also showed improved electrical properties with respect to the Au/3C-SiC system. Annealing of Pt/3C-SiC at 500°C resulted in further reduction of the leakage current and an increase of the Schottky barrier height. These changes are attributed to a consumption of the surface layer of SiC due to Pt2Si formation. However, upon annealing at higher temperatures (700°C and 900°C), a degradation of the Schottky characteristics occurred. TEM analysis showed that this degradation can be ascribed to the aggregation of carbon clusters at the interface.
This work has been supported by the European Commission in the framework of the MANSiC project (MRTN-CT-2006-035735). The authors are grateful to C. Bongiorno for his assistance during TEM sample preparation and analysis and to S. Di Franco for his help with the fabrication of Schottky diodes.
- Lebedev AA: "Heterojunctions and superlattices based on silicon carbide". Semicond Sci Technol 2006, 21: R17. 10.1088/0268-1242/21/6/R01View ArticleGoogle Scholar
- Speer KM, Neudeck PG, Crimp MA, Burda C, Pirouz P: "Possible formation mechanisms for surface defects observed in heteroepitaxially grown 3C-SiC". Phys Stat Sol A 2007, 204(7):2216. 10.1002/pssa.200675446View ArticleGoogle Scholar
- Lindefelt U, Iwata H, Öberg S, Briddon PR: "Stacking faults in 3 C -, 4 H -, and 6 H -SiC polytypes investigated by an ab initio supercell method". Phys Rev B 2003, 67: 155204. 10.1103/PhysRevB.67.155204View ArticleGoogle Scholar
- Nagasawa H, Abe M, Yagi K, Kawahara T, Hatta N: "Fabrication of high performance 3C-SiC vertical MOSFETs by reducing planar defects". Phys Stat Sol B 2008, 245: 1272. 10.1002/pssb.200844053View ArticleGoogle Scholar
- Leone S, Pedersen H, Henry A, Kordina O, Janzén E: "Thick homoepitaxial layers grown on on-axis Si-face 6H- and 4H-SiC substrates with HCl addition". J Cryst Growth 2010, 312: 24. 10.1016/j.jcrysgro.2009.10.011View ArticleGoogle Scholar
- Nagasawa H, Yagi K, Kawahara T: "3C-SiC hetero-epitaxial growth on undulant Si(0 0 1) substrate". J Cryst Growth 2002, 237–239: 1244. 10.1016/S0022-0248(01)02233-3View ArticleGoogle Scholar
- Eriksson J, Roccaforte F, Giannazzo F, Leone S, Raineri V: "Improved Ni/3 C -SiC contacts by effective contact area and conductivity increases at the nanoscale". Appl Phys Lett 2009, 94: 112104. 10.1063/1.3099901View ArticleGoogle Scholar
- Roccaforte F, La Via F, Raineri V, Calcagno L, Musumeci P: "Improvement of high temperature stability of nickel contacts on n-type 6H-SiC". Appl Surf Sci 2001, 184: 295. 10.1016/S0169-4332(01)00509-8View ArticleGoogle Scholar
- Eriksson J, Weng M-H, Roccaforte F, Giannazzo F, Di Franco S, Leone S, Raineri V: "On the viability of Au/3C-SiC Schottky barrier diodes". Mater Sci Forum 2010, 645–648: 677. 10.4028/www.scientific.net/MSF.645-648.677View ArticleGoogle Scholar
- Afanas'ev VV, Stesmans A, Bassler M, Pensl G, Schulz MJ, Harris CI: "Elimination of SiC/SiO2 interface states by preoxidation ultraviolet-ozone cleaning". Appl Phys Lett 1996, 68: 2141.View ArticleGoogle Scholar
- Giannazzo F, Roccaforte F, Raineri V, Liotta SF: "Transport localization in heterogeneous Schottky barriers of quantum-defined metal films". Europhys Lett 2006, 74: 686. 10.1209/epl/i2006-10018-8View ArticleGoogle Scholar
- Eriksson J, Weng M-H, Roccaforte F, Giannazzo F, Leone S, Raineri V: "Demonstration of defect-induced limitations on the properties of Au/3CSiC Schottky barrier diodes". Solid State Phenomena 2009, 156–158: 331. 10.4028/www.scientific.net/SSP.156-158.331View ArticleGoogle Scholar
- Schröder DK: Semiconductor Material and Device Characterization. New York: Wiley; 2006.Google Scholar
- Iucolano F, Roccaforte F, Giannazzo F, Raineri V: "Barrier inhomogeneity and electrical properties of Pt/GaN Schottky contacts". J Appl Phys 2007, 102: 113701. 10.1063/1.2817647View ArticleGoogle Scholar
- Roccaforte F, La Via F, Raineri V, Pierobon R, Zanoni E: "Richardson's constant in inhomogeneous silicon carbide Schottky contacts". J Appl Phys 2003, 93: 9137. 10.1063/1.1573750View ArticleGoogle Scholar
- Song X, Michaud JF, Cayrel F, Zielinski M, Portail M, Chassagne T, Collard E, Alquier D: "Evidence of electrical activity of extended defects in 3C-SiC grown on Si". Appl Phys Lett 2010, 96: 142104. 10.1063/1.3383233View ArticleGoogle Scholar
- Severino A, Camarda M, Scalese S, Fiorenza P, Di Franco S, Bongiorno C, La Magna A, La Via F: "Preferential oxidation of stacking faults in epitaxial off-axis (111) 3 C -SiC films". Appl Phys Lett 2009, 95: 111905. 10.1063/1.3227886View ArticleGoogle Scholar
- Eriksson J, Weng MH, Roccaforte F, Giannazzo F, Leone S, Raineri V: "Toward an ideal Schottky barrier on 3 C -SiC". Appl Phys Lett 2009, 95: 081907. 10.1063/1.3211965View ArticleGoogle Scholar
- Mohammad FA, Cao Y, Chang K-C, Porter LM: "Comparison of Pt-Based Ohmic Contacts with Ti-Al Ohmic Contacts for p -Type SiC". Jpn J Appl Phys 2005, 44: 5933. 10.1143/JJAP.44.5933View ArticleGoogle Scholar
- Kang SC, Kum BH, Do SJ, Je JH, Shin MW: "Annealing effects of Schottky contacts on the characteristics of 4H-SiC Schottky barrier diodes". Mat Res Soc Symp Proc 1999, 572: 141.View ArticleGoogle Scholar
- Na HJ, Kyeong Jeong JK, Um MY, Kim BS, Hwang CS, Kim HJ: "Effect of annealing on electrical properties of Pt/β-SiC contact". Solid-State Electron 2001, 45: 1565. 10.1016/S0038-1101(01)00167-8View ArticleGoogle Scholar
- Constantinidis G, Pecz B, Tsagaraki K, Kayambaki M, Michelakis K: "Improvements in Pt-based Schottky contacts to 3C-SiC". Mater Sci Eng B 1999, 61–62: 406. 10.1016/S0921-5107(98)00543-1View ArticleGoogle Scholar
- Papanicolaou NA, Cristou A, Gipe ML: "Pt and PtSi x Schottky contacts on n-type β-SiC". J Appl Phys 1989, 65: 3526. 10.1063/1.342626View ArticleGoogle Scholar
- Tung RT: "Electron transport at metal-semiconductor interfaces: General theory". Phys Rev B 1992, 45: 13509. 10.1103/PhysRevB.45.13509View ArticleGoogle Scholar
- Mullins FH, Brunnschweiler A: "The effects of sputtering damage on the characteristics of molybdenum-silicon Schottky barrier diodes". Solid-State Electronics 1976, 19: 47. 10.1016/0038-1101(76)90132-5View ArticleGoogle Scholar
- Calcagno L, Ruggiero A, Roccaforte F, La Via F: "Effects of annealing temperature on the degree of inhomogeneity of nickel-silicide/SiC Schottky barrier". J Appl Phys 2005, 98: 023713. 10.1063/1.1978969View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.